** Auxetic Behaviour of Re-entrant Cellular **

**Structured Kirigami at The Nanoscale **

### Jing Luo

### B.E. (Beihang University, P.R. China)

### Supervised by Prof. Qinghua Qin

### February 2017

*A thesis submitted for the degree of Master of Philosophy *

*of The Australian National University *

### Research School of Engineering

### College of Engineering & Computer Science

## To my family

**Declaration **

This thesis contains no material which has been previously accepted for the award of any other degree or diploma in any university, institute or college. To the best of the author’s knowledge, it contains no material previously published or written by another person, except where due reference is made in the text.

Jing Luo Research School of Engineering College of Engineering & Computer Science The Australian National University 28 February 2017

Signature_____________________

**Acknowledgments **

First and foremost, I would like to show endless and sincere gratitude to my primary supervisor and also the chair of my supervisory panel, Prof. Qinghua Qin, without whom my research journey would not have been possible. He has always been supportive and taught me so much about how to do high-quality research. Besides, I also would like to express my thanks and appreciation to my associate supervisor, Dr. Yi Xiao, for being so enthusiastic, supportive and helpful over my past years at the Australian National University (ANU). I will surely benefit from this unique training and experience throughout my whole life.

I am also in debt to Prof. Kun Cai, a visiting research fellow of my research group, for his advice, guidance and kindness throughout my research work and thesis manuscript writing. In addition, I am grateful to Jing Wan, an outstanding student of Prof. Cai, for his encouragements and advices on MD simulation scripts programming, too.

My sincere thanks also go to our group members for their helpful suggestions and sincere friendships throughout my research and daily life at Research Group of Engineering Mechanics, ANU. They are Prof. Hui Wang, Prof. Hongzhi Cui, Mr. Cheuk-Yu Lee, Mr. Haiyang Zhou, Mr. Song Chen, Ms. Shuang Zhang, Mr. Bobin Xing, Mr. Shaohua Yan, Ms. Yiru Ling and Ms. Ting Wang. For all of their help, interesting and valuable hints and comments.

**Abstract **

Some typical two-dimensional (2D) materials are active elements used in nano-electro-mechanical systems (NEMS) design, owing to their excellent in-plane physical properties on mechanical, electrical and thermal aspects. Considering a component with a negative Poisson’s ratio used in NEMS, the adoption of kirigamis made of periodic re-entrant honeycomb structures at the nanoscale would be a feasible method. The focus of this thesis work is to investigate the specific auxetic behaviour of this kind of structures from typical tailored 2D materials. By employing the numerical simulation method: molecular dynamics simulation, the auxetic behaviour of re-entrant cellular structured kirigami is discussed thoroughly and concretely.

selected as representative 2D materials to investigate the influence of this effect, without loss of generality.

**Contents**

**Declaration ... iii**

**Acknowledgments ... iv**

**Abstract ... vi**

**Contents ... viii**

**List of Figures ... x**

**List of Tables ... xiii**

**List of Abbreviations ... xiv**

**Chapter 1** **Introduction ... 1**

1.1 BACKGROUND AND MOTIVATION ... 1

1.2 OBJECTIVE ... 5

1.3 OUTLINE ... 6

**Chapter 2** **Literature Review ... 7**

2.1 PREVIOUS WORK ... 7

2.2 2D MATERIALS ... 8

*2.2.1* *Graphene ... 8*

*2.2.2* *Hexagonal boron nitride ... 9*

*2.2.3* *Molybdenum disulphide ... 10*

2.3 AUXETIC MATERIALS ... 11

*2.3.1* *Mechanism of auxetic materials ... 11*

*2.3.2* *Natural auxetic materials ... 13*

*2.3.3* *Artificial auxetic materials ... 17*

*2.3.4* *Properties of auxetic materials ... 20*

*2.3.5* *Applications of auxetic materials ... 21*

2.4 SUMMARY ... 23

**Chapter 3** **Research Methodology ... 24**

3.1 MD SIMULATION... 24

*3.1.1* *Modelling the N-atom physical system ... 25*

*3.1.2* *Potentials ... 26*

*3.1.3* *Time integration algorithm ... 28*

*3.1.4* *Ensembles ... 29*

*3.1.5* *Energy minimization ... 30*

*3.1.6* *Heating baths ... 30*

*3.1.7* *Periodic boundary condition ... 31*

*3.1.8* *MD software package ... 32*

*3.2.1* *Deformation control method... 33*

*3.2.2* *Stress method ... 34*

3.3 DENSITY FUNCTIONAL THEORY ... 35

3.4 THEORETICAL ANALYSIS OF RE-ENTRANT CELLULAR STRUCTURE KIRIGAMI ... 36

3.5 SUMMARY ... 38

**Chapter 4** **Size and surface effects of graphene kirigami ... 39**

4.1 MODEL DESCRIPTIONS ... 39

*4.1.1* *Geometric model of kirigami ... 39*

*4.1.2* *Methods for numerical experiments ... 41*

*4.1.3* *Schemes for size effect analysis ... 43*

4.2 NUMERICAL RESULTS AND DISCUSSIONS ... 45

*4.2.1* *Results on included angle between vertical and oblique bar varying ... 45*

*4.2.2* *Results on the width of oblique bar ... 46*

*4.2.3* *Results on different width of vertical bar ... 47*

*4.2.4* *Results on different length of vertical bar ... 48*

*4.2.5* *Results on different length of oblique bar ... 49*

4.3 SUMMARY ... 53

**Chapter 5** **Effect of different matrix 2D materials ... 55**

5.1 MODEL DESCRIPTIONS ... 55

*5.1.1* *Geometric model of kirigami ... 56*

*5.1.2* *Methods for numerical experiments ... 56*

5.2 NUMERICAL RESULTS AND DISCUSSIONS ... 57

*5.2.1* *Results on different angle between vertical and oblique bar ... 57*

*5.2.2* *Results on different width of oblique bar ... 59*

*5.2.3* *Results on different width of vertical bar ... 61*

5.3 SUMMARY ... 63

**Chapter 6** **Conclusions and Future Works ... 65**

6.1 CONCLUSIONS ... 65

6.2 LIMITATIONS... 66

6.3 FUTURE WORKS ... 67

**Bibliography ... 68**

**Publications ... 79**

**Appendix A ... 81**

**Appendix B ... 84**

**Appendix C ... 92**

**List of Figures **

Figure 1-1: Schematic diagram of different Poisson’s ratio material (a) Positive

*ν* (b) Negative *ν*. ... 2

Figure 1-2: Auxetic materials (a) Natural (b) Artificial. ... 3

Figure 1-3: Schematic diagram of tailoring 2D material to re-entrant cellular structures at the nanoscale. ... 4

Figure 2-1: Schematic diagram of graphene53. ... 9

Figure 2-2: Schematic diagram of *h*-BN53. ... 10

Figure 2-3: Schematic diagram of MoS253. ... 10

Figure 2-4: Auxetic materials exist from molecular level to macroscopic level64_{.}
... 12

Figure 2-5: Deformation mechanism of typical auxetic material. The blue dash lines represent the initial structure of this material. ... 13

Figure 2-6: Cristobalite crystal66_{ ... 13 }

Figure 2-7: Schematic diagram of cristobalite crystal. (a) Crystal structure of *α*
-cristobalite (b) The variation in Poisson’s ratio, maximum auxetic behaviour
in the (1 0 0) and (0 1 0) planes (*YZ*, *XZ*) at 45° to the major axes67. ... 14

Figure 2-8: Schematic diagram of zeolite crystal72_{. ... 15 }

Figure 2-9: Schematic diagram of zeolite crystal. (a) Crystal structure of zeolite (b) The value of Poisson’s ratio obtained from different force-field-based molecular simulations72. ... 15

Figure 2-10: The structure of B.C.C. solid metal74. ... 16

Figure 2-11: Three typical cellular structure models81_{. A: Model with re-entrant }
units, B: Model with chiral units, C: Model with rotating units. (a)
Undeformed structure and (b) Deformed structure. ... 18

Figure 2-12: (a) Microstructure details of PTFE obtained by SEM82, (b)
undeformed and deformed structure of PTFE81_{. ... 19 }

Figure 2-14: Indentation test for (a) non-auxetic and (b) auxetic materials64. ... 21
Figure 2-15: Schematic diagram of artificial blood vessels89_{. (a) Non-auxetic }

materials (b) Auxetic materials. ... 22 Figure 3-1: A schematic diagram of 3D PBC simulation box113. ... 32 Figure 3-2: A flow chart of MD simulation script programming. ... 33 Figure 3-3: A part of re-entrant cellular structured kirigami. The right half part

of (a) is a quarter of the unit cell. The grey area represents the domain
whose mechanical property is determined by the oblique bars and the
vertical bars. The vertical bars determine the mechanical property of the
yellow area. (b) The homogenised model of the right half part of (a). *E*1and

*E*2 (<*E*1) are the in-plane equivalent moduli of the yellow and grey areas,

respectively. (c) The final deformation. ... 36 Figure 3-4: Simplified homogenized zone. ... 37 Figure 4-1: Schematic diagram of graphene kirigami with detailed geometric

parameters121_{. (a) The atomic system with periodic microstructure in the }

solid yellow frame. (b) The geometry of local microstructure (in the solid yellow frame in (a)) with detailed geometric parameters of the kirigami. The microstructure has one more vertical rod than the unit cell. ... 39 Figure 4-2: The finite element model of the continuum kirigami and the local

finite element (FE) mesh in the solid black frame shown right121_{. ... 40 }

Figure 4-3: Schematic diagram of different surface energy model. ... 42 Figure 4-4: Configurations of the local microstructure of GK with different

geometric parameters in five schemes121. Here *N*(*w*) is denoted as the
number of the basic honeycomb atoms along the direction of variable w,
e.g., *N*(*w*)=3 in Figure 4-1(b). (a) Scheme 1, *θ* changes; (b) *N*(*wθ*) changes;

(c) *N*(*w*) changes; (d) *N*(*lG*) changes; (e) *N*(*lθ*) changes. ... 44

The upper figure in each case is the initial configuration after relaxation, the lower figure in each case is the final stable configuration after loading and relaxation. ... 51 Figure 4-6: Different contour plot of electron density nearby the neighbour ends

of vertical bars in the initial configuration of the pure carbon GK with (a)

*N*(*lθ*)=24 (see the upper layer of Figure 4-5(b)) and (b) *N*(*lθ*)>36 obtained by

the calculation using first principles 126_{. ... 52 }

Figure 5-1: Cell model of re-entrant cellular structured kirigami made of
different 2D materials, Graphene Kirigami, *h*-BN Kirigami and MoS2

Kirigami. For the convenience of observation, same length scale is not adopted here... 55 Figure 5-2: Configurations of local microstructure of the kirigami with different

geometric parameters in three schemes. Here *N*(*w*) is denoted as the number
of the honeycomb atoms along the direction of variable *w*, e.g., *N*(*w*) = 3 in
Figure 4-1(b). (a) Scheme 1, *θ *changes; (b) *N*(*wθ*) changes; (c) *N*(*w*)

changes. ... 56 Figure 5-3: Results on included angle between vertical and oblique bar varying.

(a) *Rp* (b) *Rm* ... 58

Figure 5-4: Results on width of oblique bar varying. (a) *Rp* (b) *Rm* ... 60

**List of Tables **

Table 4-1: Comparisons of Poisson’s ratio and the modulus ratio for the three models in Scheme 1. ... 45 Table 4-2: Comparisons of Poisson’s ratio and the modulus ratio for the three

models in Scheme 2. ... 46 Table 4-3: Comparisons of Poisson’s ratio and the modulus ratio for the three

models in Scheme 3. ... 47 Table 4-4: Comparisons of Poisson’s ratio and the modulus ratio for the three

models in Scheme 4. ... 49 Table 4-5: Comparisons of Poisson’s ratio and the modulus ratio for the three

models in Scheme 5. ... 50 Table 5-1: Comparisons of Poisson’s ratio and the modulus ratio for the three

models in Scheme 1. ... 58 Table 5-2: Comparisons of Poisson’s ratio and the modulus ratio for the three

models in Scheme 2. ... 60 Table 5-3: Comparisons of Poisson’s ratio and the modulus ratio for the three

**List of Abbreviations **

2D …… Two-Dimensional

*AIREBO * …… Adaptive Intermolecular Reactive Empirical Bond Order

*AMBER * …… Assisted Model Building with Energy Refinement

B.C.C. …… Body Centred Cubic

BK …… Hexagonal boron nitride Kirigami BP …… Black Phosphorus

CG …… Conjugate Gradient

*CHARMM * …… Chemistry at HArvard Macromolecular Mechanics

CK …… Continuum Kirigami DFT …… Density Functional Theory F.C.C …… Face Centred Cubic

FEM …… Finite Element Method
FET …… Field-Effect Transistor
*fs * …… Femtosecond

GK …… Graphene Kirigami

*GROMACS * …… GROningen MAchine for Chemical Simulations

*h*-BN …… hexagonal Boron Nitride

*LAMMPS * …… Large-scale Atomic/Molecular Massively Parallel Simulator

MD …… Molecular Dynamics

MEMS …… Micro-Electro-Mechanical Systems MK …… Molybdenum disulphide Kirigami MoS2 …… Molybdenum Disulphide

*NAMD * …… NAnoscale Molecular Dynamics

NEMS …… Nano-Electro-Mechanical Systems
*nm * …… Nanometre

*NPT * …… Isothermal–Isobaric Ensemble
*NVE * …… Microcanonical Ensemble
*NVT * …… Canonical Ensemble

PTFE …… Polytetrafluoroethylene SADS …… Sil AD Spezial

SEM …… Scanning Electron Microscope
*SW * …… Stillinger-Weber

**Chapter 1**

**Introduction **

**1.1** **BACKGROUND AND MOTIVATION**

Nowadays, auxetic materials and two-dimensional (2D) materials have been two
of the most active research fields for many years in material science1_{. Recently, }

the two formerly independent fields have started to intersect in quite new and interesting ways. Consequently, it becomes possible to some extent to take full advantages of the auxetic property in 2D materials by optimizing their microstructures, and particularly to apply the structure in the rapidly developed micro-electromechanical systems (MEMS) and nano-electromechanical systems (NEMS)2.

First of all, the 2D materials are a class of nanomaterials defined by their
property of being merely one or two atoms thick. These categories of
nanomaterials are thinned to their physical limits, and thus exhibit novel
properties different from their bulk counterpart3. These 2D materials mainly
include graphene, hexagonal boron nitride (*h*-BN) and single-layer Molybdenum
Disulphide (MoS2), etc4. Since the (re)discovery of 2D material, the single-layer

graphene, in 2004 by Novoselov and Geim5_{, they have gained extensive }

attention in a variety of fields of nano-engineering6–8, due to their remarkable
mechanical, electrical, and thermal properties9. All of these properties make 2D
materials a good candidate in the application to micro-electromechanical
systems (MEMS) and nano-electromechanical systems (NEMS)2_{. Some research }

efforts have been devoted to discovering the potential applications of the 2D
materials in the fabrication of nano-devices. As a result, they could, as raw
materials, be made into gigahertz oscillators10, nano-pumps11, nano-bearings12,
nano strain-sensors13–15_{, and many other nano-devices}16–20_{. }

.

*trans*
*axial*

ε ν

ε

= − _{ } _{(1.1) }

where *εtrans* represents transverse strain and *εaxial* represents axial strain. It
characterizes the negative ratio of the transverse normal strain to the axial
normal strain for a sample of material subjected to an axial loading22,23. When
stretched, these specific materials become thicker in the direction perpendicular
to the applied force. For illustration, Figure 1-1 intuitively presents the behavior
of different Poisson’s ratio materials under tensile test.

**Figure 1-1: Schematic diagram of different Poisson’s ratio material (a) Positive ****ν (b) Negative ν. **

As aforementioned, since the auxetic materials are able to exhibit novel
behaviour under deformation, they are of great interest in the field of material
science. Recently, the design and synthesis of such auxetic materials at the
nanoscale level is a research hotspot. For most traditional materials, the
Poisson’s ratio is typically a positive number and has a value around 0.3 in a
large number of engineering materials, such as steels. While, a lot of natural
materials have been reported to be auxetic24,25_{, they exist extensively in actual }

engineering. In Figure 1-2, the two major types of auxetic materials in the actual
engineering is shown, with the first one the natural and another fabricated from
industry, 69% of the cubic metal crystals and some face-centred cubic(F.C.C)
rare gas solids for instance behaved auxetic when they were stretched along a
non-axial direction26,27_{. As for artificial materials, there are also many auxetic }

foams29, microporous polymers30, composites31, ceramic32 and origami33. At the
nanoscale, although some auxetic material had been reported as early as twenty
years ago34_{. But, for the applications in NEMS, most of existed natural auxetic }

materials are unusable, due to their special phase form18 and length scale19.
Besides, according to the elastic strain theory35 and thermodynamics
considerations, the value of Poisson’s ratio varies mostly within -1.0 to 0.529_{, for }

the natural material. However, the wider range could be easily achieved for artificial materials by designing the specific microstructure in the matrix material.

**Figure 1-2: Auxetic materials (a) Natural (b) Artificial. **

Considering the significant demand of auxetic nano-devices in NEMS, some
artificial manufacturing technologies could be employed to fabricate this kind of
auxetic nano-devices36_{. For example, by implementing some technique methods, }

The re-entrant cellular structure is a special type of tailoring materials
with a negative Poisson’s ratio, which has been well studied by researchers for
decades25_{. An innovative tailoring method at the nanoscale is presented in the }

thesis work, which introduces the macroscopic re-entrant cellular structure into nanoscale 2D materials. In Figure 1-3, it shows how to tailor a piece of 2D material into re-entrant cellular structured kirigami at the nanoscale.

**Figure 1-3: Schematic diagram of tailoring 2D material to re-entrant cellular structures at the nanoscale. **

Due to its specific characteristics, the auxetic behaviour in a re-entrant cellular structured kirigami at the nanoscale is very important to the application in nano-devices such as NEMS. It is well known that Poisson’s ratio and modulus are the most representative mechanical properties showing auxetic behaviour. In case that an auxetic material is under tensile loading, the value of its Poisson’s ratio could govern the extent of its expansion. And the modulus ratio, which is the ratio of equivalent modulus to matrix modulus, could determine the tensile strength of auxetic materials. Therefore, studies on effects of Poisson’s ratio or the modulus ratio on materials’ mechanical behaviour may provide a guidance to the design of auxetic nano-device in NEMS. Regarding the specific microstructure of kirigami, following three major factors could affect aforementioned two mechanical properties:

(3)Matrix effect of 2D materials.

However, at nano length scale, the classical continuum mechanics theory is no longer suitable for investigating those effects on the mechanical properties of auxetic kirigami. In addition, due to the large consumptions and limitations of real experiments, there are still many essential issues remain puzzled. Here, molecular dynamics (MD) simulation, which is the most effective method for the study of mechanical behaviour at the nanoscale, is employed to study the influence of the factors discussed above.

The analysis of mechanical properties in re-entrant cellular structured kirigami in this study is expected to provide some constructive suggestions to the potential applications to nano-devices.

**1.2** **OBJECTIVE**

As discussed in Section 1.1, the innovative idea of this research work is to introduce the macroscopic re-entrant cellular structure into nanoscale structures by tailoring the single-layer 2D materials. As a result, the major objective of this work is to explore how the auxetic behaviour of tailored 2D material kirigami is affected by its geometric arrangements, surface energy and matrix 2D materials using MD simulation. Some theoretical analyses are also described to verify and illustrate the influences mentioned above.

**1.3** **OUTLINE**

**Chapter 2**

**Literature Review **

**2.1** **PREVIOUS WORK**

Materials at the nanoscale with a negative Poisson’s ratio, i.e., auxetics, are becoming increasingly popular as a result of their remarkable properties. In recent years, significant advances have been made in the design of nano-devices utilising the specific characteristics of this category of materials. These advances are either numerical or experimental.

In the respect of real experiment, the findings of artificial materials at the
nanoscale and with a negative Poisson’s ratio could be dated back to 1999, Xu et
al. used soft lithography to fabricate the auxetic materials with re-entrant cellular
microstructures40_{. Later, Hall et al. found that the in-plane Poisson’s ratio of }

carbon nanotube sheets could be tuned from positive to negative by mixing
single-walled and multi-walled nanotubes41. In 2010, Bertoldi et al. discovered
that the pattern transformations in additional curing silicone rubber Sil AD
spezial (SADS) could lead to unidirectional negative Poisson’s ratio behaviour
only under compression test42_{. By employing the contemporary advanced }

fabrication techniques, some of the materials could be made auxetic. However,
all of the aforementioned real experiments are at micrometre scale, which is
1000 times longer than nanoscale. To bypass this hurdle, a kind of kirigami at
the nanoscale is introduced here. Here, the kirigami is a variation of origami that
includes cutting of a paper43_{. It originated from Japan, where “kiru” means “cut” }

and “kami” means paper. Blees et al. used patterning methods to manipulate graphene kirigami in building robust nanoscale structures with tunable mechanical behaviour43.

the work of Blees’ experiments, researchers including Qi45, Hanakata46, Gao47
and Wei48_{, utilised MD simulations to investigate the properties of graphene }

kirigami. It can be concluded that MD simulation is a very powerful tool in the study on mechanical behaviour of nanoscale kirigami.

In this work, the macroscopic re-entrant cellular structures will be introduced at the nanoscale by tailoring the single-layer 2D material. By employing MD approach, the auxetic behaviour of this specific micro-structured materials at the nanoscale is investigated.

**2.2** **2D MATERIALS**

Many layered materials contain strong in-plane covalent bonds and weak
coupling interactions between layers. Such layered structures could be exfoliated
into individual atomic layers. Those layers with one dimension strictly limited to
one single-layer are named 2D material49_{. The background of 2D materials can }

be traced back to 2004 attributed to graphene50_{. Since then, extensive research }

efforts are dedicated to making significant progress in basic science and applications of this category of material51. The Kirigami made of 2D materials including graphene, single-layer hexagonal boron nitride and single-layer molybdenum disulphide is our focus in this thesis.

**2.2.1** **Graphene **

Among the family of 2D materials, graphene is most popular around the world. Due to generating exfoliation manufacturing method of graphene, Geim and Novoselov were awarded jointly the Nobel Prize in Physics in 201052. As a popular 2D material, the physical properties of graphene have been extensively investigated.

some desirable mechanical properties, such as large surface area, high Young’s modulus and excellent thermal conductivity.

**Figure 2-1: Schematic diagram of graphene**53_{. }

Graphene has attracted intensive attentions not only for its unusual physical properties aforementioned, but also for its potential as a basic building block for a wealth of device applications. Some examples of the structural and geometric diversity that can be achieved by using kirigami for graphene have already been demonstrated experimentally43.

**2.2.2** **Hexagonal boron nitride **

Similar to graphene, the *h*-BN has received considerable attentions too. Boron
nitride has a similar structural lattice as that found in the carbon of graphene in
that it consists of equal numbers of boron and nitrogen atoms. The *h*-BN is the
most widely used polymorph and presents the same honeycomb morphology as
graphite, with very close bond length values, being known also as the inorganic
graphite (or white graphite). It is composed of alternative boron and nitrogen
atoms in a honeycomb arrangement, as shown in Figure 2-2.

* Figure 2-2: Schematic diagram of h-BN*53

_{. }**2.2.3** **Molybdenum disulphide **

Monolayer molybdenum disulphide (MoS2) is a naturally occurring molybdenite,

[image:25.595.179.446.58.259.2]which has been studied in recent years as an alternative 2D material to graphene.
It is a kind of single-layered transition metal dichalcogenides, consisting of two
atomic layers of close-packed S atoms separated by one close-packed Mo
atomic layer55_{, which is shown in Figure 2-3. }

**Figure 2-3: Schematic diagram of MoS2**53_{. }

MoS2 exhibits many intriguing physical and chemical properties with a

wide range of potential applications. Because of its direct bandgap and its well-known properties as a lubricant, this kind of 2D material has attracted interest for diverse applications.

**2.3** **AUXETIC MATERIALS**

Auxetic materials are a kind of materials that have a unique characteristics where they would expand laterally when stretched, or shrink laterally when they are compressed. Following subsections would discuss the mechanism of auxetic materials and some typical auxetic materials.

**2.3.1** **Mechanism of auxetic materials **

When a material is uniaxially loaded in tension, it extends in the direction of the
applied load, which extension is accompanied by a lateral deformation. The
lateral deformations are quantified by a property known as the Poisson’s ratio
which is defined in mathematical terms as the negative ratio of the transverse
over longitudinal strains, as mentioned in equation(1.1). In particular, for
stretching in the *x-*direction, the Poisson’s ratio in the *xy *plane of the material is
defined by equation(1.1):

.

*y*
*xy*

*x*

ε ν

ε

= (2.1)

Even though, the value of Poisson’s ratio was always assumed to be
positive since most everyday materials get thinner when stretched. Today, it has
been shown through numerous studies that negative Poisson’s Ratio materials
exist, meaning that referring to Figure 1-2(b), for the *xy* plane, a uniaxial load in
the *x-*direction results in an extension in the *y-*direction. The existence of these
materials confirms what had been predicted by theory for a long time, the
classical theory of elasticity23 states that the Poisson’s ratio for
three-dimensional isotropic materials may range between -1≤*ν*≤0.529, while for
two-dimensional isotropic materials, it may range between -1≤*ν*≤156_{, with no upper }

Up to now, a lot of auxetic materials have been discovered, the negative
Poisson’s behaviour could be revealed by the intrinsic of the micro or
nanostructure of the materials and the way that this geometric arrangement
deforms on the tensile test. In fact, there are various geometric arrangements
based deformation mechanisms presented to illustrate the auxetic behaviour in
different natural occurring auxetic materials, including cubic metal crystals26_{, }*α*_{}

-cristobalite60_{ and liquid crystalline polymers}61_{ and in different artificial auxetic }

materials, such as micro/nanostructured polymers62_{ and foams}63_{. Auxetic }

behaviour is scale independent and the similar combination of geometry and deformation mechanism can operate at any length scale level. Figure 2-4 shows various discovered auxetic materials at different length scale level.

**Figure 2-4: Auxetic materials exist from molecular level to macroscopic level**64_{. }

**Figure 2-5: Deformation mechanism of typical auxetic material. The blue dash lines represent the initial **

**structure of this material. **

It should be mentioned that many natural materials have been found to be auxetic in the practical engineering65. In the category of artificial or man-made materials, auxetic materials are also popular.

**2.3.2** **Natural auxetic materials **

*2.3.2.1* *Cristobalite *

A popular naturally-occurring auxetic is the *α*-cristobalite, which has attracted a
lot of attentions in recent years. The cristobalite is a sort of mineral that has a
high-temperature of silica, which means that it shares same chemical formula
with quartz, SiO2. This kind of crystalline consists of two phases, one is with

high-temperature phase (*α*-cristobalite) and the other is with low-temperature
phase (*β*-cristobalite)58,66_{. Figure 2-6 shows the crystal structure of cristobalite }

Looking at the example of cristobalite in Figure 2-7, the auxetic behaviour has been measured in single crystalline form. It's anisotropic in different extent at different place and the signs of Poisson’s ratio in different directions are presented.

**Figure 2-7: Schematic diagram of cristobalite crystal. (a) Crystal structure of ****α-cristobalite (b) The ****variation in Poisson’s ratio, maximum auxetic behaviour in the (1 0 0) and (0 1 0) planes (YZ, XZ) at 45° to **

**the major axes**67_{. }

Interestingly, for the *α*-cristobalite, when doing the averaging to come up
with a polycrystalline aggregate Poisson’s ratio, an overall isotropic auxetic
material is ended up. In Figure 2-7(a), the unit crystal structure of *α*-cristobalite
is shown. It has been reported that the extent of auxeticity in the unit single
crystal is such that isotropic polycrystalline aggregates of *α*-cristobalite are also
generated to exhibit a negative Poisson’s ratio. Figure 2-7(b) shows the range of
Poisson’s ratio obtained from the experiments of *α*-cristobalite60_{. }

*2.3.2.2* *Zeolite *

Zeolite is another kind of important naturally-occurring auxetic material. It is a type of microporous and aluminosilicate mineral, which is commonly used as commercial adsorbents and catalysts. Zeolites are aluminosilicate framework structures containing molecular-sized cages and channels formed from an array of corner-sharing SiO44- and AlO45- tetrahedral. Figure 2-8 shows the structure of

**Figure 2-8: Schematic diagram of zeolite crystal**72_{. }

Due to its highly geometric nanostructures in the crystal structure, auxetic behaviour of zeolite would be easy to generate. In Figure 2-9(a), the unit crystal structure of zeolite is shown. The negative Poisson’s ratio could be to some extent explained by a simple geometry-deformation mechanism relationship. It should be mentioned there are very few experimental data available on the single crystalline mechanical properties of zeolite. The value of its Poisson’s ratio derived from different force-field-based molecular simulations is listed in Figure 2-9(b), which ranges from -0.55 to -0.33.

**Figure 2-9: Schematic diagram of zeolite crystal. (a) Crystal structure of zeolite (b) The value of Poisson’s **

**ratio obtained from different force-field-based molecular simulations**72_{. }

**Force-field**

*ν*

_{xy}*ν*

_{yx}### Burchart

68### -0.55

### -0.55

### BKS

69### -0.33

### -0.53

### Universal

70### -0.33

### -0.40

[image:30.595.85.547.465.717.2]*2.3.2.3* *Cubic metals *

Some metals may exhibit auxetic properties as they are stretched or compressed
in certain direction. For instance, Baughman reported that up to 69% of all cubic
materials and some face-centred cubic rare gas solids behaved auxetic when
they were stretched along the [110] off-axis direction73,74_{. Figure 2-10 shows a }

typical cubic metal possessing a negative Poisson’s ratio.

**Figure 2-10: The structure of B.C.C. solid metal**74_{. }

closes part of the rhombus, by making atoms 5 and 6 apart and approach to a
negative *ν*(110,110).

Many other natural auxetic materials may exist in the real world. Due to the limitation of space, however, we won’t go further on the discussion in this area.

**2.3.3** **Artificial auxetic materials **

Although some natural auxetic materials have been reported recently, artificial auxetic materials are also very popular in the practical engineering. They can be classified into following types, cellular structure, microporous structure and composites.

*2.3.3.1* *Auxetic cellular structure *

In the cellular structure, there are various honeycomb models which could show
auxetic characteristics. Some models have re-entrant units or chiral units, and
some have rotating units. Figure 2-11 shows three typical cellular structure
models. For re-entrant units structure in honeycomb, the first traditional one was
first reported by Gibson in 198275_{. When a stress load is applied in either }

direction, hereby the diagonal ribs move in such a way, which leads to the
auxetic effect in the other direction. Next, in terms of the chiral type, the word
“chiral” means non-superimposable on the mirror image76,77. The auxetic
behaviour is owing to the rotation of rigid rings, which makes ligaments on the
rings wind or unwind, hereby obtaining this unique characteristic78_{. Finally, in }

**Figure 2-11: Three typical cellular structure models**81_{. A: Model with re-entrant units, B: Model with }

**chiral units, C: Model with rotating units. (a) Undeformed structure and (b) Deformed structure. **

Due to its remarkable property and special microstructure, re-entrant cellular units are adopted to achieve negative Poisson’s ratios of 2D materials in this work.

*2.3.3.2* *Auxetic microporous structure *

ultra-high molecular weight polyethylene (UHMWP) is another well-known
microporous polymer83_{. Figure 2-12 shows the scanning electron micrograph }

(SEM) of PTFE and mechanism of its auxetic behaviour.

**Figure 2-12: (a) Microstructure details of PTFE obtained by SEM**82_{, (b) undeformed and deformed }

**structure of PTFE**81_{. }

Under the uniaxial tension, the fibrils of the microporous structure rotate with respect to the connection of the nodules and the overall structure then undergoing expansion. Hence, microporous structure possesses auxetic properties, because their porous structures allow sufficient space for the nodules to spread apart.

*2.3.3.3* *Auxetic Composites *

It is well known that continuum materials with specific microstructural
characteristics and composite structures have been confirmed to be auxetic
analytically84_{. To an extent, some composites could exhibit auxetic behaviour by }

**Figure 2-13: A periodic fibre reinforced composite with star-shaped encapsulated inclusions**86** _{. }**
In summary, there are still a lot of other artificial auxetic materials developed by
scientists and technicians. However, due to limitation of space, no more
discussions are presented here.

**2.3.4** **Properties of auxetic materials **

As aforementioned, auxetic materials possess enhanced properties, owing to the counterintuitive characteristics subjected to the applied stress load. A lot of theoretical analyses and experiments have shown that mechanical properties can be reinforced by auxeticity87. Materials with a negative Poisson’s ratio have the following special properties:

(1)High in-plane indentation resistance; (2)Good fracture toughness;

(3)High transverse shear modulus; and, (4)High dynamic properties, etc.

*2.3.4.1* *Indentation Resistance *

**Figure 2-14: Indentation test for (a) non-auxetic and (b) auxetic materials**64_{. }

For that reason, auxetic materials are more resistant to indentations than traditional materials.

*2.3.4.2* *Facture toughness *

Compared with traditional materials, auxetic materials have other special and
desirable mechanical properties87_{. For example, once the material has a crack, it }

expands and closes up the crack, after being stretched apart. That is to say, this kind of material should have more resistance to fracture. Besides, it also has high material resistance to shear strain.

*2.3.4.3* * Dynamic properties *

Some foam structures with a negative Poisson’s ratio exhibit an overall
superiority regarding damping and acoustic properties, compared with the
conventional ones63_{. Their dynamic crushing performance is superior to normal }

foams, indicating that a potential application in structural integrity compliant elements.

**2.3.5** **Applications of auxetic materials **

(1)Unique negative Poisson’s ratios; (2)Superior mechanical properties; and (3)Acoustic absorption properties.

The Poisson’s ratio affects deformation kinematics in various ways, some of them are useful and could influence the distribution of stress.

*2.3.5.1* *Sensors *

Since the low bulk modulus of auxetic materials makes them more sensitive to hydrostatic pressure, they can be adopted in the design of hydrophones or other precision sensors. Due to the high in-plane indentation resistance, the sensitivity of sensor made by auxetic materials is increased by almost one order of magnitude, compared with traditional ones88.

*2.3.5.2* *Biomedicine *

In the area of clinical application, the man-made blood vessel is a representative use for the biomedicine. As shown in Figure 2-15, if the blood vessel in a human body is made from auxetic materials, the wall would become thicker when a pulse of blood flows through it. Otherwise, the wall thickness would decrease, when the blood vessel is made from conventional materials.

**Figure 2-15: Schematic diagram of artificial blood vessels**89_{. (a) Non-auxetic materials (b) Auxetic }

Besides, some more potential applications, such as surgical implants90, and
suture anchors or muscle/ligament anchors, where the porous structure could
contribute to promoting bone growth89_{. }

*2.3.5.3* * Aerospace and defence *

Some structures with the unique properties of auxetic materials (i.e. negative
Poisson’s ratio) have already been adopted in real military defense applications.
For example, a kind of pyrolytic graphite (*ν*=-0.21) has been employed for
thermal protection in aerospace area91_{. And some large single crystals of Ni}

3Al

(*νmin*=-0.18) has been used in Vanessa for aircraft gas turbine engines74_{. }

**2.4** **SUMMARY**

**Chapter 3**

**Research Methodology **

In nano length scale, since the walls becoming more dominant, the classical
continuum mechanics theory breaks down gradually. Besides, due to the huge
consumption in experiments, there are still a lot of important questions remain
unsolved. Thus, the numerical simulation may provide an alternative approach
that could help to circumvent these problems. MD simulation is the most
common method for the study of mechanical behaviour at the nanoscale because
of relatively high accuracy, low computational cost92–94_{. Simulations at different }

length scale considering different physics require different simulation methods. To study the mechanical behaviour, MD simulation and molecular mechanics are used to calculate the mechanical deformation of different 2D materials.

**3.1** **MD SIMULATION**

In recent years, computational engineering have been extensively developed for
different length scales and material properties. In this work, the length scale
spans from nano to macro, and MD simulation is one of the most powerful tools
for computational mechanics study. MD simulation was first introduced by
Berni Alder for transition problem in 195792, and afterwards it was developed
for various studies in physics, biology, chemistry, material science and
nano-mechanics. MD computes time evolution of a cluster of interacting atoms by
integrating their equations of motions. The classical molecular dynamics is
employed here, and the word “classical” represents particles in simulation
system respects the classical mechanics, in other words, Newton’s Laws95_{, are }

followed:

,
*i* *i*

*m*

=

**i**

**F** **a** (3.1)

For the atom *i* in a *N*-atom-system, where *mi *is the atom’s mass,

2 2 ,

*i*
*i*

*d*
*dt*

= **r**

The term **a***i* is the acceleration, and **F***i* is the force acting on the atom. Thus and

so, the force is derived as the gradients of potential with respect to atomic displacements:

### (

1,### )

.*i*

*i* = −∇**r***V* *N*

**F** **r r** (3.3)

Therefore, MD simulation is a deterministic method: given initial
positions and velocities, the **F***i* following time evolution is completely

determined and the computer calculates a trajectory in a *6N*-dimensional phase
space (*3N *positions and* 3N *momenta). Besides, the MD simulation is a type of
statistical mechanics method which contains a set of distributions according to
determined statistical ensembles. Physical quantities could be easily evaluated
by taking the arithmetic average among different instantaneous values during the
MD simulation. In the limit of long simulation time, the phase space could be
regarded as fully sampled, and all the mechanical properties would be generated
during the averaging process. In summary, the MD simulation can be applied in
to calculate mechanical properties of microstructure made of different 2D
materials.

**3.1.1** **Modelling the N-atom physical system **

The major part of a MD simulation is the physical model, which means selecting
the potential in simulation: a function, *V*(**r***1*,…,**r***N*). Forces are then derived from

the equation(3.3), which implies the conservation of total energy, and term *V* has
been simply written as a sum of pairwise interactions.

When it comes to the practical use, various types of many-body potentials
are now very popular in condensed matter simulation, because the
approximation has been recognized to be inadequate. The improvement of
discovering accurate potentials is remarkable, which includes the development
of Adaptive Intermolecular Reactive Empirical Bond Order (*AIREBO*)
potential96,97_{, }_{Tersoff}_{ potential}98–100_{ and Stillinger-Weber (}_{SW}_{) potential}101,102_{, }

related to single-layer MoS2; and *Tersoff* potential is involved in the MD

simulation on the single-layer *h*-BN.

**3.1.2** **Potentials **

In general, materials acquire their properties from the interactions among their
component atoms103_{. These basic interactions maintain the atoms congregate in a }

specific crystalline structure. The same interactions also define how the atoms prefer to arranging themselves on the surface or around a vacancy.

In order to build an appropriate model for MD simulation, the potential
function is required to describe the potential energy and force fields for the
whole system. The potential function is to model the interactions between
particles (atoms, molecules and proteins, etc.), and all electron interactions are
lumped into the potential form. It usually takes an empirical description where
the parameters are fitted from more accurate Density Functional Theory (DFT)
calculations or real experiments. The general analytic form of an intramolecular
potential is originally derived by Abell from chemical pseudopotential theory104_{. }

Beginning with a local basis of unperturbed atomic orbitals, Abell shows that chemical binding energy can be simply written as a sum of nearest neighbours:

### ( )

### ( )

.*R* *A*

*bonding* *ij* *ij* *ij*

*i* *j i*

*E* *V* *b V*

≠

=

### ∑∑

_{}

**r**−

**r**

_{}(3.4)

The functions *VR*_{(}_{r}_{) and }_{V}R_{(}_{r}_{) are pairwise interactions that denote all }

interatomic repulsion and attraction from valence electrons. The quantity *bij*

denotes a bond order between atoms *i *and *j* that is derived from electronic
structure theory. As mentioned in Subsection 3.1.1, three major potentials are
our focus in this thesis, which are *AIREBO*, *Tersoff* and *SW * potential,
independently.

*3.1.2.1* * AIREBO potential *

hydrogen atoms96. The *AIREBO* potential consists of three terms and could be
written as：

, , ,

1

. 2

*REBO* *LJ* *TORSION*

*ij* *ij* *ijkl*

*i* *j i* *k i j l i j k*

*E* *E* *E* *E*

≠ ≠ ≠

= _{} + + _{}

### ∑∑

### ∑ ∑

(3.5)All of three terms are included in the simulation by default. The *EREBO*

term gives the model its reactive capabilities and only describes short-ranged
*C-C*, *C-H* and *H-H* interactions. The *EREBO*_{ term adds longer-ranged interactions by }

using a form similar to the standard Leonardo Jones potential. And the cutoff of

*C-C* is 0.34 nm, with a scale factor of 3.0, the resulting *ELJ* cutoff would be
1.02nm. The *ETORSION*_{ term denotes an explicit }_{4}_{-body potential that describes }

various dihedral angle preferences in hydrocarbon configurations.

*3.1.2.2* *Tersoff potential *

The *Tersoff* potential computes *3*-body potential and its analytical form for the
pair potential:

### ( ) ( )

### ( )

1 2 ,*ij*

*i* *j i*

*ij* *C* *ij* *R* *ij* *ij* *A* *ij*

*E* *V*

*V* *f* *f* *b f*

≠

=

= _{} + _{}

### ∑∑

**r** **r** **r**

(3.6)

where the function *fC*(**r**) denotes a cutoff term, which ensures only
nearest-neighbour interactions, functions *fR*(**r**) and *fA*(**r**) are competing attractive and
repulsive pairwise terms, describes the *2*-body interaction and the *3*-body
interaction respectively. In addition, quantity *bij* is the bond angle term. The
hybrid *B-N-C* *Tersoff* potential105_{ is adopted in this thesis. More details of this }

potential refer to Appendix A.

*3.1.2.3* *SW potential *

Recently, researchers have selected the *SW* potential developed by Jiang in
2015106, for the simulation on single-layer MoS2. The *SW * style potential

computes a *3*-body potential for the total energy. The total energy interactions in

,

*total* *LJ* *two* *three*

*E* =*E* +*E* +*E* (3.7)

where the *Etwo* term denotes all *2*-body interactions with all possible pairs, i.e.

*Mo-S*, *Mo-Mo* and *S-S*:

( max)

### (

### )

/ 4

/ 1 ,

*r r*
*two*

*E* = *Ae*ρ − *B r* − (3.8)

And *Ethree* term covers the atoms involved in the *ϕ*, *θ* and *ψ* angles:

( ) ( )

_{(}

_{)}

1/ 12 max 12 2/ 13 max 13 2

0

cos cos .

*r* *r* *r* *r*

*three*

*E* =*Ke*ρ − +ρ − θ − θ (3.9)

It is noted that the *ELJ *only takes effect when there are two or more layers
of MoS2 in simulation models and it denotes the *van der Waals* interaction

between S atoms in a different layer of multilayers MoS2. More details of this

potential refer to Appendix A.

**3.1.3** **Time integration algorithm **

It is well known that the time integration algorithm is the most powerful
numerical method to integrate the equations of motion of the various interacting
particles and following their trajectory. The basic theory of time integration
algorithm is finite difference methods, where time is discretised on finite small
time step, *∆t*. Once the positions, velocities and accelerations of particles are
given, the integration algorithm could derive all of these quantities at the later
time.

In nanoscale MD simulation, one of the most commonly used time integration algorithms is the Verlet algorithm107,108:

### (

### )

### ( ) (

### ) ( )

2### ( )

42 .

*t*+ ∆ =*t* *t* − *t*− ∆ +*t* *t* ∆ +*t* *O* ∆*t*

**r** **r** **r** **a** (3.10)

This is the basic form of Verlet algorithm, where **a**(*t*) is just the acceleration,
which is the force divided by the mass:

### ( )

*t*

*V*

### ( )

### ( )

*t*.

*m*

∇

= − **r**

**a** (3.11)

Despite the fact that algorithm is simple in use, as well as it is very
accurate and stable in the simulation, the problem with this kind of version is
that velocities are not generated directly. To eliminate this weakness, a better
version of the same algorithm is developed, named the velocity Verlet
algorithm. In this version of the algorithm, the positions, velocities and
accelerations at time *t*+*∆t* are derived from the same quantities at the time *t* as
following:

### (

### ) ( ) ( )

### ( )

### ( )

### ( )

### (

### )

### (

### (

### )

### )

### (

### )

### (

### )

2 1 , 2 1 , 2 2 1 , 1 . 2 2*t* *t* *t* *t* *t* *a t* *t*

*t*

*t* *t* *t* *t* *t*

*t* *t* *V* *t* *t*

*m*
*t*

*t* *t* *t* *t* *t* *t*

+ ∆ = + ∆ + ∆
∆
_{+} _{=} _{∆ +} _{∆}
+ ∆ = − ∇ + ∆
∆
+ ∆ = _{} + _{}+ + ∆ ∆

**r** **r** **v**

**r** **v** **a**

**a** **r**

**v** **v** **a**

(3.12)

It is noted that if one wants to save 3*N* positions, velocities and
accelerations, 9*N *memory is occupied, but there is no need to simultaneously
store the values at two different times.

**3.1.4** **Ensembles **

In MD simulation, a statistical ensemble is required to control some quantities
related to the thermodynamics, like pressure, temperature and energy.
Traditional MD simulation differs from most other experimental studies is that
the energy and volume are fixed, instead of temperature and pressure94_{.Common }

ensembles consist of canonical ensemble (*NVT*), micro-canonical ensemble
(*NVE*) and isothermal-isobaric ensemble (*NPT*). MD simulation produces *NVE*

ensemble averages, while constant-temperature experiment is comparable to the

*NVT* ensemble; suppose constant pressure is maintained as well, it is the *NPT*

ensemble.

**3.1.5** **Energy minimization **

In the field of MD simulation, energy minimization is the process of discovering a stable arrangement in space of a congregation of atoms, according to the second law thermodynamics. Performing an energy minimization of the simulation system is to adjust atoms positions iteratively. The objective function being minimized is the total potential energy of the system as a function of the

*N*-atom coordinates:

### (

### )

### ( )

### ( )

### (

### )

### (

### )

### (

### )

### ( )

1 , , , , , , , , , , , , , , , , , , , , , ,*N* *pair* *i* *j* *bond* *i* *j* *angle* *i* *j* *k*

*i j* *i j* *i j k*

*angle* *i* *j* *k* *l* *improper* *i* *j* *k* *l* *fix* *i*

*i j k l* *i j k l* *i*

*E* *E* *E* *E*

*E* *E* *E*

= + + +

+ +

### ∑

### ∑

### ∑

### ∑

### ∑

### ∑

**r** **r** **r r** **r r** **r r r**

**r r r r** **r r r r** **r**

(3.13)

where the first term is the sum of non-bonded pairwise interactions, the second to fifth terms are bond, angle, dihedral and improper interactions respectively, and the last term is a supplementary term to equation.

Due to its high computational efficiency, Conjugate Gradient (CG)
algorithm often used in an atomistic simulation. Hence, CG algorithm is utilized
in this thesis for minimizing the whole simulation system110_{. The CG algorithm }

mainly depends on the atomic forces and atomic energy. And it goes through a series of search directions. The local minimum energy point along each search direction is reached before algorithm proceeding to the next search.

**3.1.6** **Heating baths **

The reliability of simulations significantly depends on an appropriate modelling of the interaction with thermal reservoirs. In a study of the non-equilibrium process, stationary non-equilibrium states are required to reach, by that to obtain the relevant determined thermodynamic properties. In order to gain the stable simulation, the reservoirs on both sides are linear, however, the central system is nonlinear.

theorem. Taking the case of one-dimension chain for example, this equals to the following form of Langevin equations:

### (

1### )

### (

1### ) (

### )

1### (

### )

,*i i* *i* *i* *i* *i* *i* *i* *i* *iN*

*m***r** =*F* **r** −**r**− −*F* **r**+ −**r** + ξ+−λ+**r** δ + ξ−−λ−**r** δ (3.14)
where *ξ+* and *ξ- *denote independent variables respecting Wiener processes with
zero mean and variance 2λ_{±}*K T _{B}*

_{±},

*KB*is the Boltzmann constant and

*T*

_{±}means the temperature of two different heating reservoirs.

For the sake of providing a self-consistent description of
out-of-equilibrium processes, definitive heating baths have been introduced, among
which the Nosé-Hoover thermostat has been employed by most of researchers in
the MD simulation111,112_{.}

In the heating bath, the evolution of the particles is controlled by the following equation:

### (

1### )

### (

1### )

, i S , , i S

*i*

*i* *i* *i* *i* *i*

*i*

*m* *F* *F* ς

ς
+ +
− +
− −
∈
= − − − _{− }
∈
**r**

**r** **r** **r** **r** **r**

**r**

(3.15)

where ς± are supplementary variables which model the microscopic behaviours
of the thermostat, and *S*_{±}stand for two sets of *N*_{±} particles onto reservoirs.

**3.1.7** **Periodic boundary condition **

**Figure 3-1: A schematic diagram of 3D PBC simulation box**113_{. }

**3.1.8** **MD software package **

Nowadays, there are a lot of popular MD simulator software are implemented in
the research fields, such as *LAMMPS*, *GROMACS*, *CHARMM*, *AMBER*, *NAMD*

and *MD++*, etc.

In this work, MD simulations were conducted with the open source code
package *LAMMPS*. *LAMMPS* is a classical molecular dynamics code, and an
acronym for Large-scale Atomic/Molecular Massively Parallel Simulator114_{. It is }

**Figure 3-2: A flow chart of MD simulation script programming. **

**3.2** **STRAIN CALCULATION IN 2D MATERIAL KIRIGAMI**

In this thesis, one of the most important mechanical quantities derived from MD simulations is the strain calculation in 2D material kirigami. Based on the continuum mechanics theory, there are two different methods were used to calculate strain field of single-layer 2D material kirigami from atomistic simulation results. The deformation control method and stress method are discussed as followings.

**3.2.1** **Deformation control method **

method, the strain increment with a constant strain rate is applied to simulation
model every constant time step115_{. }

In the uniaxial tensile test, the engineering (nominal) strain and stress are related by the following equations:

0
0
,
*xt* *x*
*x*
*x*
*L* *L*
*L*

ε = − (3.16)

0
0
,
*yt* *y*
*y*
*y*
*L* *L*
*L*

ε = − (3.17)

0

0 0 0

1
,
*x*
*x*
*x* *y*
*U*
*V*

*V* *l* *l* *T*

σ ε ∂ = ∂ = ⋅ ⋅ (3.18)

where *lx0* and *ly0* are the initial lengths of nanoribbon in *x*- and *y*-directions, *lxt *

and *lyt* are the lengths of the nanoribbon after deformation, term *U* denotes the
strain energy, term *V0* is the initial volume of the simulation model and term *T* in
the equation means the assumed thickness of given 2D materials. Hence, the
equivalent Young’s modulus *Eequiv* and Poisson’s ratio *ν* are defined as follows:

2
2
0 0
1
,
*x*
*equiv*
*x*
*U*
*E*

*V* ε _{ε} _{=}

∂
=
∂ (3.19)
.
*y*
*x*
ε
ν
ε

= − (3.20)

In *LAMMPS*, the strain-control method is utilized by changing the volume
or shape of the simulation box during a dynamics run. Besides, engineering
strain rate could be maintained by using this method.

**3.2.2** **Stress method **

### (

### )

### (

### )

1 , 1 , .*xx* *xx* *yy*

*yy* *yy* *xx*

*xy*
*xy*

*E*
*E*

*G*

ε σ µσ

ε σ µσ

σ ε = − = − = (3.21)

However, it is noteworthy that, since the relationship between stress and
strain is assumed to be linear, then the resulting strain could be mostly
underestimated, especially at large deformation117_{. }

The virial stress calculation consists of both potential and kinetic parts. Moreover, the plane stress constitutive model was utilized to calculate the strain by the equations of

1
0
1
0 ,
1
0 0
2
*xx* *xx*
*yy* *yy*
*zz* *zz*
*E* *E*
*E* *E*
*G*
µ
ε σ
µ
ε σ
ε σ
_{−}
_{} _{}
_{= −}_{} _{}_{⋅}
_{} _{}
_{} _{}
_{} _{}
(3.22)

It is noted that the values output from *LAMMPS* are in units of

“Pressure∙Volume”. Accordingly, the real value of stress should take the “Volume” factor into calculation.

In general, the resultant strain is required in this research work, rather than stress distribution. In addition, in order to better control and measure the rate of applied stretched strain. The first method, which is deformation-control method, is utilized here.

**3.3** **DENSITY FUNCTIONAL THEORY **

electron being present at a specific location. In quantum chemical calculations,
the electron density, *ρ*(**r**) is a function of the coordinates **r**, thus **r**∙*ρ*(**r**) is the
number of electrons in a small value. The function *ρ*(**r**) could be written as:

### ( )

*P*

_{µν µ}

### ( ) ( )

_{ν},

µ ν

ρ **r** =

### ∑∑

φ**r**φ

**r**(3.23)

where, *P* denotes the density matrix and *ϕ* represents basic function.

**3.4** **THEORETICAL ANALYSIS OF RE-ENTRANT CELLULAR STRUCTURE **
**KIRIGAMI**

To estimate the mechanical behaviour of re-entrant cellular structure kirigami, a theoretical analysis is developed as following. As shown in Figure 3-3, the right part with yellow and grey areas (including adjacent bars) is a quarter of the unit cell of kirigami. We noticed that the equivalent mechanical properties, equivalent modulus and Poisson’s ratio, are determined by the mechanical and geometric parameters of the oblique and vertical bars.

[image:51.595.86.538.455.656.2]Suppose that the total strain along *y*-direction, *εy* is specified and denote
the equivalent moduli of yellow and grey areas as *E1* and *E2*, respectively.
Besides, the area fraction of the two areas are *w*1 and *w*2= (1-*w*1), respectively.

**Figure 3-3: A part of re-entrant cellular structured kirigami. The right half part of (a) is a quarter of the **

**unit cell. The grey area represents the domain whose mechanical property is determined by the oblique **

**bars and the vertical bars. The vertical bars determine the mechanical property of the yellow area. (b) **

The structure shown in Figure 3-3(b) could be further simplified as the structure shown in Figure 3-4.

**Figure 3-4: Simplified homogenized zone. **

According to the composite materials theory118_{, the equivalent modulus of }

the kirigami could be easily obtained as

1 2
1 2
1
,
*equiv*
*w* *w*

*E* = *E* +*E* (3.24)

then the equivalent modulus could be represented by *Eequiv*=*E*1∙*E*2/(*E*1∙*w*2+*E*2∙*w*1).

Let *εy*1 and *εy*2 represent the line strains of the yellow and grey parts along *y*

-direction, respectively. *εy* could be then written as:
1 *y*1 2 *y*2 *y*,

*w*ε +*w*ε =ε (3.25)

and the total resultant force along *y*-direction applied to yellow and grey parts is
the same:，

1 1 2 2.

*y* *y* *y*

*F* =*E* ⋅ε =*E* ⋅ε (3.26)

Making use of equations (3.25) and (3.26), the *εy*1 and *εy*2 could be expressed in

terms of *εy* as:

1

1 2 1 2

2

2 1 2 1

1
/
.
1
/
*y* *y*
*y* *y*

*w* *w E* *E*

*w* *w E* *E*

ε ε
ε ε
_{=}
_{+} _{⋅}
_{=}
+ ⋅
(3.27)

1 2,

*x* *x* *x*

*l*
*w*

*l* *w* *l* *w*

θ

θ θ

ε = ⋅ε + ⋅ε

+ + (3.28)

where *εx*<0 is the *x*-strain of the vertical bar adjacent to the yellow part, *εx*2

denotes the *x*-strain of the grey part. For the structure with small deformation, it
can be obtained using the following formulation,

2
2 2
1
cot .
*G*
*x* *y*
*l*
*w*

*w* *l*_{θ}

ε ≈ε ⋅ ⋅ θ (3.29)

Therefore, the equivalent Poisson’s ratio could be written as

2 1

2 1 2 1

1 1

~ cot .

1 / /

*x* *x*

*p*

*y* *y*

*w*
*R*

*w l*_{θ} *w* *w E* *E* *l*_{θ}

ε _{θ} ε

ε ε

= − ≈ − _{} ⋅ + _{}

+ _{} + ⋅ _{} (3.30)

By employing the theoretical analysis developed in this section, the size effect of re-entrant cellular structure kirigami could be illustrated clearly.

**3.5** **SUMMARY**

In summary, MD simulations are conducted within the Sandia-developed open
source code *LAMMPS*114. The Verlet algorithm is used for simulation time
integration with a time step of 0.5*fs*, and different ensembles are applied to the
given physical situations. For the potential aspects, interactions between carbon
atoms are described by the *AIREBO* potential96_{ with a cutoff at 1.02nm, which }

has been adopted to measure the mechanical properties of carbon-based
nanostructures119,120. And the force field to describe interactions between Mo
and S atoms is a modified version of SW potential developed by Jiang106_{, in }

2015. Besides, the interactions between B and N atoms in *h*-BN are set to be
*B-N-C* *Tersoff* potential105_{. All the simulations are carried out at 8K with }

**Chapter 4**

**Size and surface effects of graphene kirigam**

**i**

**4.1** **MODEL DESCRIPTIONS**

Strictly speaking, some typical 2D materials, such as graphene and black
phosphorus, are not auxetic materials, or not in-plane auxetic more precisely,.
For example, they are either out-of-plane auxetic24,65_{, or wrinkle-open-up }

auxetic38. Once a kirigami of 2D material is tailored into a re-entrant cellular structure, the auxetic behaviour will be generated. The size and surface effects on the performance are of importance and are our focus in this chapter.

**4.1.1** **Geometric model of kirigami **

Figure 4-1 shows the schematic diagram of kirigami tailored from the 2D material. The size effect is mainly due to the five main variables in the cell honeycomb structure, which are,

**Figure 4-1: Schematic diagram of graphene kirigami with detailed geometric parameters**121_{. (a) The }

**atomic system with periodic microstructure in the solid yellow frame. (b) The geometry of local **

**microstructure (in the solid yellow frame in (a)) with detailed geometric parameters of the kirigami. The **

**microstructure has one more vertical rod than the unit cell. **

(1)*θ*, the internal angle between vertical bar and oblique bar;
(2)*wθ*, the width of oblique bar;